APPUCA nONS OF INFRARED PHOTOACOUSTIC
SPECfROSCOPY FOR WOOD SAMPLES)
Department of Forestry
10- State Univenity
Ames, IA 500 II
John F. McClelland, Siquan Luo,2
Po-Liang Chien,2 R. D. Walker2
Physicist, Visiting Scholar, Postdoctoral FeUow, Postdoctoral Fellow.
Ames laOOratory' u.s. Des-nJDeDt of Enerv
Ames, IA SOO II
Various infrared (IR) spectroscopic techniques for the analysis of wood samples are briefty discussed.
Theories and instrumentation of the newly developed photoacoustic spectroscopic (PAS) technique
for measurina absorbance spectra of solids are presented. Some important applications of the PAS
technique in wood science ~ are discussed. The application of the Fourier transfonn in~-
photoacoustic spectroSCOpic (FTlR-PAS) technique is demonstrated by three preliminary studies of
diff~nt fonns of wood samples.
K~rds: Infrared spectroscopy, photoacoustic spectroscopy, wood sections, macerated wood ele-
ments, decayed wood samples.
Infrared spectroscopy is an indispensable method for both qualitative and quan-
titative analysis of organic substances. Various infrared spectroscopic techniques
have been used to study solid wood and the various constituents of wood (Liang
et aI. 1960; Harrington et aI. 1964; Bolker and Somerville 1963; Sarkanen et aI.
I Joumai Paper No. J-12S9S of the Iowa Aariculture and Home Economics Experiment Station
(Project No. 2606), Ames, Iowa. This study was partly supponed by Southern Forest Experiment
Station, U.S. Forest Service, under cooperative agreement No. 19-83-040.
1 Present addreues are: (S.L) University of Science and Technology of Cbin8, Hefei. Anhui, PRC;
(C.LC.) Advance Fuel R~. 81 01~ St.. East Hartfoni, CT 06108; and (RD. W.) Florida [)cpt.
of Environmental Regulation. 26 Blair Stone Rd.. Ta1Iaba~. A. 32399.
S The Ames Laboratory is operated for the U.S. Department of EDerIY by Iowa State University
under Contract No~ W-140S-Eng-82. This research was supported partly by the Division of Chemical
Sciences, Office of Enerwy Research and partly by the Assistant Secretary for Fossil Eneqy throUlh
the PittsbUJ1b EDerIY TechnolOlY Center.
WDOdGlld FI6fr.sc ~I), 1911, ~ 132-14S
0 1988 by die Society 01 Wood SciIDce ad T~
Southern Forest Experiment Station
Pineville, LA 71360
(Received Febniary 1987)
133KIlO et 41. - INFRARED PHOTOACOUSTIC SPECTROSCOPY OF WOOD
1967) and to elucidate the mechanisms of delignification processes during pulping
(Michell et al. 1965; Marton and Sparks 1967) and of aging processes of wood
surfaces (Chow 1971; Feist and Hon 1984). Recently, because of increasing interest
in the chemical pretreatment of wood to improve wood adhesion, infrared spec-
troscopy has been employed to investigate the mechanisms of chemical activation
of wood surfaces and adhesive bond formation (Jenkin 1976; Rammon et al.
1982; Phillippou and Zavarin 1984).
The use of conventional infrared spectroscopic techniques for the analysis of
solid samples presents some severe problems, including the opaqueness and light-
scattering properties of samples and the low sample-to-noise signal available from
dispersive instruments. With the advent of the commercial Fourier Transform
Infrared (FTIR) instruments and different accessories, infrared spectra of solid
samples can be obtained more rapidly with greater sensitivity. In this paper,
various infrared spectroscopic techniques for the analysis of wood and wood
component samples are briefly discussed, with the major emphasis being to in-
troduce the newly developed Photoacoustic Spectroscopic (PAS) technique. The
capability and potential of the FTIR-PAS technique for the analysis of wood
samples is demonstrated by some exploratory experiments.
INFRARED SPECTROSCOPIC TECHNIQUES FOR WOOD SAMPLES
Light scattering and high optical density render the direct transmission spec-
troscopic analysis of wood samples very difficult. Light scattering can be greatly
reduced by either impregnating thin wood sections with, or dispersing finely milled
wood samples in, Nujol. Nujol, however, has interfering absorption bands at 2,850
to 3,000, 1,486, 1,379, and 720 cm-l. Inorganic halides, when pressed into thin
pellets, are an alternative that have a high transmittance throughout the midin-
frared region. Therefore, transmission spectroscopic analysis of wood samples
can be studied by embedding or dispersing them in halides such as KBr and KCI.
Liang et al. (1960) and Harrington et al. (1964) found that a thin wood section
embedded in KBr gave a better IR spectrum than milled wood dispersed in a
KBr pellet. The latter group of authors also found that pressing several thin wood
sections in a KBr pellet gaye a sharper spectrum than using a single wood 5ection.
There are situations, however, when wood sections are either difficult to obtain
or relatively opaque such that wood samples must be studied in the form of fine
powder dispersed in KBr pellets. Transmission spectroscopic analyses of isolated
wood components, especially hemicelluloses and lignins, are generally studied by
dispersing them in KBr pellets or Nujol.
With a careful control of sample concentration in KBr pellets and with a double
beam spectrophotometer, it is possible to obtain difference spectra between sets
of two different samples. For example, employing this technique, Bolker and
Somerville (1963) were able to find differences between lignins in wood and pulp
and isolated lignins.
Attenuated total reflectance (ATR) technique
An important method called attenuated total reflection (A TR) or internal re-
flection spectroscopy (IRS) for obtaining the inftared spectra of solids has been
WOOD AND FlBER SCIENCE, JANUA.V 1988. V. 20(1)134
described by Fahrenfort (1961). Initial A TR devices used a single-reflection prism
and a variable angle of incidence to produce the desired spectra. Attenuated total
reflection spectra can be markedly improved by using a multiple-reflection prism
such as KSR-S. By placing a sample in very close contact with the reflecting
surface of the prism, the energy that escapes temporarily from the prism is selec-
tively absorbed by the sample. The spectrum of the internally reflected radiation
is very similar to a typical transmission spectrum. The infrared band intensities
are the equivalent of a shallow (approximately 5 IJ.m or less) penetration into the
sample and are completely independent of the sample thickness.
The A TR technique has been succesfully used to study undisturbed wood sur-
faces (Hse and Bryant 1966; O'Brian and Hartman 1969) and solid-phase changes
of wood and wood components during chemical treatments (O'Brian and Hartman
1971; Jenkin 1976). Marton and Sparks (1967) also successfully used the ATR
technique to determine the lignin content of unbleached kraft and sulfite pulps
and uncoated paper samples.
In the A TR technique, the amount of infrared absorption is dependent on the
area and efficiency of a close optical contact between the sample and the prism.
Therefore, the intensity of absorption of a sample with an uneven and rough
surface such as a wood section is a function of pressure applied to assemble the
sample onto the prism. Thus, the pressure dependence of the A TR spectra is the
main disadvantage of using the technique to study solid wood samples.
Diffuse reflectance technique
With the advent of the commercial Fourier transfonn spectrometers, diffuse
reflectance spectroscopy has become an important method for qualitative and
quantitative analysis of solid samples. In Diffuse Reflectance Infrared Fourier
Transfonn Spectroscopy (ORIn), a powdered sample is usually intimately mixed
with an alkali halide powder such as KBr or KCI. When the powder matrix is
irradiated, IR radiation is diffusely scattered in all directions. By a special optical
arrangement, part of the diffuse radiation is refocused and directed to the detector.
The ratio of the spectrum containing the sample to a KBr or KO reference
spectrum yields the diffuse reflectance spectrum of the sample, which is similar
to the transmission spectrum of the sample measured in a KBr or KCl pellet. In
some cases, diffuse reflectance spectra of neat samples can be measured.
Schultz et al. (1985a) found that the lignin, gluc~e, and xylose contents of
wood determined by the DRIFT technique gave highly significant correlations with
values obtained by conventional chemical analyses. Thus, the more rapid DRIFT
technique can be used to analyze solid lignocellulosic materials with reasonable
accuracy. The DRIFT technique has also been used to estimate degree of crys-
tallinity of a variety of celluloses (Schultz et al. 1985b).
One of the major factors influencing diffuse relectance spectra is the particle
size of the sample and the matrix material. Because the optical density is reduced
with smaller sample particles, the sharpness and the relative intensity of absorption
bands in a diffuse reflectance spectrum increase with decreasing particle siu.
Therefore, it is necessary to standardize particle size in any particular series of
measurements (Krishnan 1984).
135KIlO et aJ. - INFRAREDPHOTOAOOUSTIC SPECfROSCOPV OF WOOD
Photoacoustic Sample Cell
FIG. 1. Schematic of the photoacoustic spectroscopy technique (reprodured with permission from
PHOTOACOUSTIC SPECfRosroPY OF SOUDS